reaction diffusion in the nickel-chromium-aluminum .reaction diffusion in the...
Post on 01-Sep-2018
Embed Size (px)
N A S A TECHNICAL NOTE
REACTION DIFFUSION I N THE NICKEL-CHROMIUM-ALUMINUM A N D COBALT-CHROMIUM-ALUMINUM SYSTEMS
NATIONAL AERONAUTICS AND SPACE ADMINISTRATION WASHINGTON, D. C. FEBRUARY 1977
TECH LIBRARY KAFB, NM
- 7. Key Words (Suggested by Author(sJ)
Diffusion; Nickel alloys; Cobalt alloys; Pro- tective coatings; Gas turbines
- -~ - - 1. Report No. 2. Government Accession No.
NASA T N D-8383 4. Tit le and Subtitle
REACTION DIFFUSION IN THE NICKEL-CHROMIUM- ALUMINUM AND COBALT-CHROMIUM-ALUMINUM SYSTEMS
18. Distribution Statement Unclassified - unlimited STAR Category 26
7. Aut l -x(s)
Stanley R. Levine
19. Security Classif. (of this report)
9. Performing Organization Name and Address NASA Lewis Research Center and U.S. Army Air Mobility R & D Laboratory Cleveland, Ohio 44135
National Aeronautics and Space Administration Washington, D. C. 20546
12. Sponsoring Agency Name and Address
20. Security Classif. (of this page) 21. NO. of Pages 22. Rice'
Unclassified 66 A04
0134090 3. necipient s wra iog NO.
5. Report Date February 1977
6. Performing Organization Code
8. Performing Organization Report No.
E-8835 10. Work Unit No.
505- 01 11. Contract or Grant No
13. Type of Report and Period Covered
Technical Note 14. Sponsoring Agency Code
15. Supplementary Notes
16. Abstract The effects of MCrAl coating-substrate interdiffusion on oxidation life and the general multi- phase, multicomponent diffusion problem were examined. Semi-infinite diffusion couples that had sources representing coatings and sinks representing gas turbine alloys were annealed at 1000, 1095O, 1150, or 1205' C for as long as 500 hours. The source and sink aluminum and chromium contents and the base metal (cobalt or nickel) determined the parabolic diffusion rate constants of the couples and predicted finite coating lives. The p source strength concept pro- vided a method (1) for correlating p recession ra te constants with composition; (2) for determin- ing reliable average total, diffusion, and constitutional activation energies; and (3) for calcu- lating interdiffusion coefficients.
REACTION DIFFUSION IN THE NICKEL-CHROMIUM-ALUMINUM
AND COBALT-CHROMIUM-ALUMINUM SYSTEMS
by Stanley R. Levine
Lewis Research Center and U. S. Army A i r Mobil ity R&D Laboratory
Physically vapor-deposited overlay coatings based on the Ni- Cr-A1 o r Co- Cr- A1 (M-Cr-A1) systems a r e used in the aircraft gas turbine industry because they give better oxidation, hot corrosion, and thermal fatigue protection to turbine airfoils than do aluminide coatings. The oxidation life of a protective coating is controlled by aluminum consumption caused by alumina spalling, erosion, and interdiffusion with the substrate. The relative rates of these processes are determined by coating and substrate composi- tion, service environment, and temperature.
The purposes of this study were (1) to determine the effect of coating and substrate chemistry on the kinetics of interdiffusion and their relation to diffusion- zone constitu- tion and (2) to develop a procedure for analyzing diffusion in multicomponent, multiphase systems. Semi-infinite diffusion couples that had MCrAl sources representative of coatings and sinks representative of nickel- or cobalt-base gas turbine alloys were assembled and annealed at 1000, 1095O, 1150, or 1205' C for as long as 500 hours. The couples were examined by optical microscopy; Knoop microhardness traverses and layer growth measurements were also made.
specific sink composition since changes in source aluminum content a re more important than changes in chromium content. Sink composition is as important as source compo- sition in determining p recession kinetics in diffusion couples and life in finite coatings. Nickel-base alloys a r e more stable sources and stronger sinks than cobalt-base alloys. Total and diffusion activation energies were determined from layer growth constants. By introducing the concept of p source strength, which is determined from the appropri- ate phase diagrams, the Wagner solution for consumption of a second phase in a semi- infinite couple was successfully applied to the analysis of the MCrAl couples. This provided a method (1) for correlating p recession rate constants with couple composition; (2) for determining reliable average total, diffusion, and constitutional activation ener- gies; and (3) for calculating interdiffusion coefficients.
Parabolic growth constants can be correlated with source aluminum content for a
The physically vapor-deposited overlay coatings base$ on the Ni-Cr-A1 (ref. 1) o r Co-Cr-A1 systems are gaining acceptance in the aircraft gas turbine industry because they give better oxidation, hot corrosion, and thermal fatigue protection to turbine air- foils and have a higher temperature capability than the widely used diffusion aluminide coatings (ref. 2). With higher-use-temperature substrates such as directionally solidi- fied eutectics (ref. 3) and oxide-dispersion-strengthened alloys (ref. 4), the aluminide coatings that successfully protect conventional superalloys offer inadequate diffusional stability. And so the use of overlay coatings is no longer a matter of choice.
mined by the rate at which aluminum is depleted by alumina spalling and erosion and by interdiffusion with the substrate. The relative rates of these processes a re determined by the coating and substrate compositions and by the service environment and tempera- ture. In the case of aluminide coatings, the diffusion reaction between the coating and the substrate has been shown to be far more important than oxidation in determining coating life at l l O O o C (ref. 5). It appears that the diffusion reaction is also important in the depletion of overlay coatings, but to a lesser degree. This is based on the follow- ing qualitative argument: Typically, overlay coatings are about twice as thick as alumi- nide coatings (0.013 cm for overlays vs 0.006 cm for aluminides) and have about half the aluminum content on a weight percent basis (12 MO for overlays vs 25 to 30 eo for aluminides). If we assume that reduction of the surface aluminum content by 50 percent constitutes aluminum reservciir depletion, the coating's diffusion life t can be computed from the coating thickness h and the interdiffusion coefficient D by
The oxidation life of a protective coating in the gas turbine environment is deter-
h2 t = - D
(ref. 6) t o a first rough approximation. The depletion criterion seems to be a reason- able one for both coating systems based on the results of Pettit (ref. 7) and Wallwork and Hed (ref. 8). According to Pettit, alloys in the Ni-A1 system become spinel formers at about 14-wt% aluminum. Wallwork and Hed found that below about 5-f10 aluminum the NiCrAl and CoCrAl alloys no longer form a continuous protective layer of A1203. From equation (1) it is apparent that the double thickness of the overlay coatings could result in a fourfold increase in life over simple aluminide coatings, assuming equal diffusion coefficients. In the Ni-A1 system the interdiffusion coefficient is a func- tion of the phase under consideration and its particular chemistry. For example, Janssen (ref. 9) reports that at l l O O o C the interdiffusion coefficient for Ni3A1 is 3 . 6 ~ 1 0 - ~ O cm2/sec; the interdiffusion coefficient for the saturated terminal nickel solid
2 solution varies with the source phase from 2 . 6 ~ 1 0 - ~ ' cm /sec with a yf (Ni3Al) source to 5. 7x10-10 cm2/sec with a P (NiA1) source; and the interdiffusion coefficient for 62-at.%-Ni NiAl is 2 . 7 ~ 1 0 - ~ cm2/sec. For degradation of an aluminide coating (p ) it is reasonable to select the interdiffusion coefficient for p when computing life from equa- tion (1). With an overlay coating the constitution of the diffusion zone is a function of coating and substrate chemistry and can be either y, y ' , or a mixture of the two. An
2 interdiffusion coefficient of 4. 5x10-10 cm /sec is a reasonable average value to use when estimating life for an overlay coating from equation (1). Consequently, one might expect the typical overlay coating to have more than 20 times the life of the typical simple aluminide. A factor of 2 or 3 in life for each coating class may result from variations in diffusivity caused by alloy and coating chemistry.
Alternatively coating life may be improved by controlling the constitution of the diffusion zone through control of coating chemistry and its interaction with alloy chem- istry. There is more latitude for accomplishing this with overlay coatings since wide variations in coating chemistry can be readily made.
This study had several purposes. One was to examine the effect of overlay coating chemistry and substrate chemistry on the kinetics of coating depletion by interdiffusion. An associated second purpose was to examine the effect of coating and substrate chem- is t ry on diffusion- zone constitution and mechanical properties. An additional purpose of this study was to develop a procedure for analyzing diffusion in multicomponent, multiphase systems. were assembled from cast NiCrAl and CoCrAl alloys and annealed at 1000, 1095', 1150, or 1205' C for as long as 500 hours. The couples were examined by optical microscopy, and Knoop microhardness traverses and layer growth measurements were made. Alloy constitution was established from optical metallography assisted in some instances by the energy dispersive X-ray spectroscopy (EDS) fea